Concrete pavement design, construction, and performance
Concrete Pavement Design,
Construction, and Performance
Also available from Taylor & Francis
Reynolds’s Reinforced Concrete Designer Handbook
T. Threlfall et al. Hb: ISBN 978–0–419–25820–9
Pb: ISBN 978–0–419–25830–8
Reinforced Concrete 3rd edn
P. Bhatt et al. Hb: ISBN 978–0–415–30795–6
Pb: ISBN 978–0–415–30796–3
P. Mondorf Hb: ISBN 978–0–415–39362–1
Concrete Mix Design, Quality Control and
Specification 3rd edn
K. Day Hb: ISBN 978–0–415–39313–3
Binders for Durable and Sustainable Concrete
P.-C. Aïtcin Hb: ISBN 978–0–415–38588–6
Aggregates in Concrete
M. Alexander et al. Hb: ISBN 978–0–415–25839–5
Concrete Pavement Design Guidance Notes
G. Griffiths et al. Hb: ISBN 978–0–415–25451–9
Information and ordering details
For price availability and ordering visit our website www.sponpress.com
Alternatively our books are available from all good bookshops.
Concrete Pavement Design,
I dedicate this book to my late father, Norbert
Delatte Sr., who taught me to love books.
List of Figures ix
List of Tables xiii
1 Introduction 1
2 Types of concrete pavements 25
3 Performance 46
4 Subgrades, subbases, and drainage 69
5 Selection of concrete materials 95
6 Mixture design and proportioning 111
7 Design fundamentals 129
8 Highway pavement design 155
9 Light duty pavement design 172
10 Airport pavement design 199
11 Industrial pavement design 221
12 Transitions, special details, and CRCP reinforcement 231
13 Subgrade and subbase construction 249
14 Paving 262
15 Finishing, texturing, curing, and joint sawing and sealing 279
16 Concrete pavement maintenance 306
17 Rehabilitation 315
18 Overlays and inlays 330
1.1 Dowel and tie bar baskets placed in preparation for
slipform paving (photo courtesy of The Great Lakes
Construction Company, Hinckley, Ohio). 7
1.2 (a) and (b) Slipform pavers (photo courtesy of The Great
Lakes Construction Company, Hinckley, Ohio). 8
1.3 Finishing slipformed pavement around a banked curve
(photo courtesy of The Great Lakes Construction
Company, Hinckley, Ohio). 9
2.1 Jointed plain concrete pavement (JPCP) (courtesy:
2.2 Jointed reinforced concrete pavement (JRCP) (courtesy:
2.3 Continuously reinforced concrete pavement (CRCP)
(courtesy: ACPA). 29
2.4 Dowel basket assembly with corrosion resistant
epoxy-coated dowels (photo by author). 31
2.5 Doweled joint (FAA 2004: 86, 86–1). 32
2.6 Tie bar basket assemblies with corrosion resistant
epoxy-coated tie bars – dowel baskets are also shown
(photo by author). 33
2.7 Longitudinal joint (FAA 2004). 34
2.8 Header and dowel basket for a transverse construction joint
(photo by author). 34
2.9 Expansion joint detail (FHWA 1990a). 36
2.10 RCC pavement construction – Columbus, Ohio (photo by
2.11 Permeability of a pervious pavement demonstration
project – Cleveland, Ohio (photo by author). 45
3.1 Corner breaks (ACPA 1996a: VIII-16). 47
3.2 High severity D-cracking (Miller and Bellinger 2003: 37). 49
3.3 High severity longitudinal crack (Miller and Bellinger
2003: 39). 50
3.4 High severity transverse crack in JRCP (Miller and
Bellinger 2003: 41). 50
3.5 High severity transverse joint spalling (ACPA 1996a:
3.6 Map cracking (Miller and Bellinger 2003: 48). 53
3.7 Scaling (Miller and Bellinger 2003: 48). 54
3.8 Polished aggregate surface (Miller and Bellinger 2003: 49). 55
3.9 Blowup (Miller and Bellinger 2003: 52). 56
3.10 Faulted transverse joint (photo by author). 57
3.11 Water bleeding and pumping (Miller and Bellinger 2003: 58). 60
3.12 High severity punchout (Miller and Bellinger 2003: 79). 61
4.1 Roadway geometry inputs for concrete pavement drainage
4.2 Computation of inflow. 88
4.3 Determining the permeability of the base. 89
4.4 Designing the base by the depth-of-flow method. 89
4.5 Checking the base design by the time-to-drain method. 90
4.6 User-defined subgrade material. 91
4.7 Checking need for a separator layer. 91
4.8 Edge-drain design. 93
5.1 Combined aggregate relationship (coarseness factor) chart
(courtesy: Shilstone and Shilstone 2002). 102
6.1 Comparison of PCA 1984 and StreetPave fatigue
7.1 Curling stress correction factors for a finite slab (after
Bradbury 1938). 133
7.2 Corner, edge, and interior loading. 135
7.3 Maximum joint spacing based on slab thickness D
and modulus of subgrade reaction k for L/ ≤5 0 in
(a) U.S. customary units and (b) metric units. 144
8.1 WinPAS solution to design problem. 162
8.2 Spreadsheet solution to AASHTO 1998 design example. 164
8.3 Spreadsheet faulting check for AASHTO 1998 design. 165
8.4 Sensitivity analysis for AASHTO 1998 design. 166
9.1 StreetPave traffic major arterial traffic category. 178
9.2 StreetPave life cycle cost module input screen. 181
9.3 Design example traffic inputs. 182
9.4 Design example pavement inputs. 183
9.5 Concrete pavement design. 184
9.6 Design example fatigue and erosion table. 185
9.7 Rounding considerations. 185
9.8 Sensitivity of slab thickness to k-value. 186
9.9 Quadrant construction at an urban intersection in
Cleveland, Ohio (photo by the author). 196
10.1 FAA R805FAA.xls rigid airport pavement design
10.2 FAA R805FAA.xls rigid airport pavement design
spreadsheet frost design. 211
10.3 FAA R805FAA.xls rigid airport pavement design
spreadsheet computation of composite k-value. 212
10.4 Determining critical aircraft. 213
10.5 LEDFAA basic input screen. 214
10.6 Sample rigid pavement section from the LEDFAA
samples file. 215
10.7 Aircraft traffic mix. 216
10.8 Example problem rigid pavement section as designed. 218
11.1 RCCPave vehicle library. 224
11.2 RCCPave design results for example 1. 226
11.3 RCCPave design inputs for example 2. 227
12.1 Combination chair and transverse steel detail
1 in = 25 4 mm (FHWA 1990b). 243
12.2 Lug anchor treatment 1 in = 25 4 mm 1 ft = 305 mm
(FHWA 1990b). 245
12.3 Recommended WF steel beam terminal joint design
1 in = 25 4 mm 1 ft = 305 mm (FHWA 1990b). 247
14.1 Slipform paving train (ACPA 1996a: VI-6). 264
14.2 Concrete pavement produced by slipforming (ACPA
1996a: VI-6). 265
14.3 Stringline and paver sensing wand (ACPA 1996a: VI-15). 266
14.4 The pad line (ACPA 1996a: VI-20). 267
14.5 Vibrators (ACPA 1996a: VI-26). 268
14.6 Dowel basket (ACPA 1996a: VI-88). 269
14.7 Dowel bar inserters (ACPA 1996a: VI-32). 270
14.8 CRCP steel installation with tube feeders (ACPA 1996a:
14.9 Fixed form paving (ACPA 1996a: VI-68). 272
14.10 Steel forms for fixed form paving (ACPA 1996a: VI-72). 273
14.11 Blockouts for utility, drainage, and similar structures
(ACPA 1996a: VI-91). 274
15.1 Transverse tining to provide macrotexture (ACPA 1996a:
15.2 Burlap drag to provide microtexture (ACPA 1996a: VI-53). 280
15.3 Transverse joint initial and widening cut (ACPA 1996a:
15.4 Properties of rough asphalt concrete subbase. 301
15.5 Concrete mixture proportions. 302
15.6 Construction inputs. 303
15.7 Environmental inputs. 304
15.8 Results of analysis. 304
15.9 Evaporation rate predictions. 305
16.1 Effect of delay in applying a maintenance treatment. 307
16.2 Falling weight deflectometer (photo by the author). 310
17.1 Hole prepared for a full depth repair at a joint (ACPA
1996a: VIII-28). 317
17.2 Partial depth repair (ACPA 1996a: VIII-57). 318
17.3 Full depth repair with dowels and fiberboard for isolation
(ACPA 1996a: VIII-41). 320
17.4 Dowel bar retrofit (ACPA 1996a: VIII-66). 323
17.5 Diamond grinding (ACPA 1996a: VIII-11). 325
17.6 Grout injection for slab stabilization (ACPA 1996a:
18.1 Joint mismatching (Smith et al. 2002: 4–9). 333
18.2 Lane widening options (Smith et al. 2002: 4–12). 334
18.3 Unbonded overlay on two lanes with a third lane paved at
the same time (photo courtesy: Dale Crowl). 335
18.4 A transition detail for bridge approaches and overpasses
for unbonded overlays (Smith et al. 2002: 4–13). 335
18.5 Saw cutting for whitetopping with ruts (figure courtesy:
ACPA, Smith et al. 2002: 5–12). 343
18.6 A transition detail for bridge approaches and overpasses
for whitetopping (figure courtesy: ACPA, Smith et al.
2002: 5–9). 343
18.7 Output of ACPA UTW calculator
18.8 UTW placed as an inlay (photo by the author). 347
18.9 Failure of UTW by panel sliding (photo by the author). 348
18.10 UTW-thickened end transition detail (figure courtesy:
ACPA, Smith et al. 2002: 6–7). 349
4.1 Recommended k-value ranges for various soil types
(adapted from Hall et al. 1997: 80, AASHTO 1998: 6) 72
4.2 Effect of untreated subbases on k-values (PCA 1984: 6) 75
4.3 Effect of cement-treated subbases on k-values (PCA 1984: 6) 75
4.4 Effect of untreated subbases on k-values (FAA 2004: 15) 75
4.5 Effect of stabilized subbases on k-values (FAA 2004: 57) 76
4.6 Conditions where no subbase is required (FAA 2004: 55,
Table 3.10) 77
6.1 Sample concrete mixture designs for early opening to traffic
(Van Dam et al. 2005: A-1–A-2) 127
7.1 Dowel bar diameter recommendations (ACPA 1998: 27,
ACI Committee 2002 325: 15) 149
7.2 Tie bar spacing recommendations in mm (in) 152
8.1 Reliability and standard normal deviate ZR (AASHTO
1993, I-62 and II-9) 158
8.2 Drainage coefficients Cd (AASHTO 1993, II-26) 159
8.3 Load transfer coefficients J by pavement type (AASHTO
1993, II-26) 159
8.4 Input values for design example (AASHTO 1993, II-45) 161
8.5 Sensitivity analysis – effect of design parameters on
thickness D 162
9.1 Street and parking lot traffic classifications from ACI
325.12R-11 and ACI-330R-6 (ACI Committee 325 2002:
11, ACI Committee 330 2001: 6) 174
9.2 StreetPave traffic categories from help file 177
9.3 Traffic categories – axles per 1000 trucks 179
9.4 Pavement thickness design tables, aggregate interlock joints,
no edge-support 187
9.5 Pavement thickness design tables, aggregate interlock joints,
supported edges 190
9.6 Pavement thickness design tables for pervious concrete 192
10.1 Landing gear type conversion factors (FAA 2004: 25) 203
10.2 Forecast traffic and equivalent annual departures (FAA
2004: 26) 203
10.3 Maximum joint spacing for unstabilized base (FAA
2004: 87) 207
10.4 FAA dowel bar recommendations (FAA 2004: 88) 208
10.5 Traffic mix for LEDFAA design example 217
12.1 AASHTO CRCP percent steel design example (AASHTO
1993 II-56–II-62) 238
12.2 Recommended longitudinal reinforcement sizes (FHWA
12.3 Recommended WF beam dimensions (FHWA 1990b) 246
15.1 Joint sealing materials (ACPA 1996a: VII-32) 292
15.2 Typical values for PCC CTE (modified from AASHTO
1993: II-29) 294
15.3 Typical values for PCC coefficient of shrinkage
(modified from AASHTO 1993: II-29) 294
There are too many people to thank for helping me with this book, but I
will try anyway. To begin with, the members of American Concrete Insti-
tute Committees 325, Concrete Pavements, Committee 327, Roller Com-
pacted Concrete Pavements, Committee 330, Concrete Parking Lots and Site
Paving, and Committee 522, Pervious Concrete, have helped me consider-
ably with discussions during committee meetings and over beers afterward.
James Shilstone, Sr. (Jim) and James Shilstone, Jr. (Jay) supplied material
for Chapter 5, and Juan Pable Covarrubias supplied material for Chapter 9.
Tim Smith of the Cement Association of Canada, Dale Crowl of the Ohio
Department of Transportation, and George Palko of The Great Lakes Con-
struction Company supplied photographs. In addition to my colleagues, I’d
like to thank my students in courses at Cleveland State University and at
the University of Alabama at Birmingham over the years, because teaching
them challenged me to research and synthesize the material. Finally, I need
to thank my wife Lynn and our children, Isabella and Joe, for their patience
while I was drafting this manuscript.
Figures 2.1, 2.2, 2.3, and 18.7 are reprinted by permission of the Ameri-
can Concrete Pavement Association, Skokie, IL.
Figures 3.1, 3.5, 14.1–14.11, 15.1–15.3, 17.1–17.6, and Table 15.1 are
reprinted from course materials developed by the American Concrete Pave-
ment Association and used in National Highway Institute (NHI) training.
NHI is a part of the Office of Professional and Corporate Development,
Federal Highway Administration.
Concrete pavements have been used for highways, airports, streets, local
roads, parking lots, industrial facilities, and other types of infrastructure.
When properly designed and built out of durable materials, concrete pave-
ments can provide many decades of service with little or no maintenance.
“Concrete generally has a higher initial cost than asphalt but lasts longer
and has lower maintenance costs” (Hoel and Short 2006: 26).
In some cases, however, design or construction errors or poorly selected
materials have considerably reduced pavement life. It is therefore impor-
tant for pavement engineers to understand materials selection, mixture
proportioning, design and detailing, drainage, construction techniques, and
pavement performance. It is also important to understand the theoretical
framework underlying commonly used design procedures, and to know the
limits of applicability of the procedures.
The first concrete pavement was built in Bellefontaine, Ohio, in 1891, by
George Bartholomew. He had learned about cement production in Germany
and Texas and found pure sources of the necessary raw materials, limestone
and clay, in central Ohio. Because this was the first concrete pavement,
the city council required him to post a $5,000 bond that guaranteed the
pavement would last 5 years. Over 100 years later, part of his pavement
was still in use. Details of the history of the project are provided by Snell
and Snell (2002).
The American Concrete Pavement Association (ACPA) “100 Years
of Innovation” website (http://www.pavement.com/PavTech/AbtConc/His-
tory/Introduction.html) notes that the pavement “was an immediate success.
Local businessmen petitioned to have the entire block around the Square
paved with concrete. In 1893, Court Avenue and Opera Street were paved.
Columbus Avenue and the remainder of Main Street followed in 1894.” At
that time, the term “concrete” was not yet in general use, so the material
was called “artificial stone” and mixed by hand in 1.5 m (5 ft) square
forms. Other early concrete pavements included Front Street in Chicago,
which was built in 1905 and lasted 60 years, and Woodward Avenue in
Detriot (1909) which was the first mile of concrete pavement.
There may have been even earlier concrete pavement experiments. Pasko
(1998) notes “according to Blanchard’s American Highway Engineers’
Handbook of 1919, in 1879 in Scotland, a concrete was used with port-
land cement for binding. ‘The surface was very good, but when the road
commenced to break, it went to pieces very fast.’ Blanchard goes on to say
that the first portland cement concrete (PCC) pavement in the United States
was put down in 1893 on South Fitzhugh Street in Rochester, N.Y., by
J.Y. McClintock, Monroe county engineer. This was a section of portland
cement grouted macadam, a forerunner of the modern concrete pavement
of the Hassam type. The cost of this pavement was $1 per square yard
(per 0.84 square meters). However, the pavement soon deteriorated.” In
spite of this possible earlier history, it is clear the Bellefontaine was the first
successful, long-lasting concrete pavement.
In 1913, 37 km (23 miles) of concrete pavement was built near Pine Bluff,
Arkansas, at a cost of one dollar per linear foot. It became known as the
“Dollarway.” The pavement was 2.7 m (9 ft) wide and 125 mm (5 in) thick.
The remains of Dollarway are preserved as a rest area along US 6. This was
followed, in 1914, by 79 kms (49 miles) of concrete pavement for rural county
roads in Mississippi, and by the end of 1914, a total of 3,778 km (2,348 miles)
of concrete pavement had been built in the United States (ACPA 2006).
Despite the growing importance of the automobile, it was in fact a bicy-
clists’ association that was organized and effective enough to press for the
passage of the first Federal-Aid Highway Act in 1916. In the same year, the
Portland Cement Association was organized to promote the use of portland
cement and concrete. The concrete industry paved “seedling miles” with
the hope that the public would demand they be linked together with more
Early road tests
To supplement theory in the quest to develop design procedures for con-
crete pavements, many road tests were held over the years. It is believed
that the first controlled evaluation of concrete pavement performance was
conducted in 1909 by the Public Works Department of Detroit. Steelshod
shoes and heavy iron wheels were mounted at opposite ends of a pole,
revolving around a circular track, to simulate horse and wagon traffic of
the day. Test sections included concrete, granite, creosote block, and cedar
block. Based on this study, Wayne County, Michigan paved Woodward
Avenue with concrete and then paved sixty more miles of concrete roads in
the following 2 years (ACPA 2006).
After 1916, concrete roads were being built 125–225 mm (5–9 in) thick,
but little was known about thickness requirements. During 1912–1923,
the State of Illinois conducted the Bates Road Test. Using old World War
I trucks with wheel loads from 454 to 5,900 kg (1,000 to 13,000 lbs),
traffic was applied to test sections of different materials and thicknesses.
The concrete sections of uniform cross-section were 100–225 mm (4–9 in)
thick while thickened-edge sections were 229-125-229 mm and 229-152-
229 mm (9-5-9 and 9-6-9 in), some with edge bars. The results showed
that of the 22 brick, 17 asphalt, and 24 concrete sections in the test, one
brick, three asphalt, and 10 concrete sections satisfactorily withstood the
truck loadings. As a result, several design formulations were developed for
Illinois to use in building its first state highway system (ACPA 2006). The
Bates Road Test provided basic data that was used by design engineers for
many years (Yoder and Witczak 1975: 4).
Until 1922, many pavements had been built with no joints and a thick-
ened center section in an attempt to prevent the formation of an erratic
longitudinal crack that developed in 4.9–5.5 m (16–18 ft) wide pavements.
Based on the results of the Bates Road Test, center joints to eliminate
longitudinal cracking were adopted (ACPA 2006).
Other road tests followed. The Pittsburg, California Road Test of 1921–
1923 compared reinforced concrete pavement to plain concrete (ACPA
2006). This test showed no particular advantage to reinforcement, but the
test pavements were built without joints and did not reflect modern practice
(Ray 1981: 5).
In 1950 and 1951, the Bureau of Public Roads (now FHWA) with the
Highway Research Board (now the Transportation Research Board),
several states, truck manufacturers, and other highway-related indus-
tries conducted Road Test One – MD just south of Washington, D.C.
An existing 1.1 mi (1.8 km) of two-lane highway was carefully invento-
ried, instrumented, and traversed by 1,000 trucks per day. The results
showed the value of good load transfer between slabs, the effects of
speed and axle weights, and the problems caused by pumping. It pro-
duced the first dynamic wheel equivalence factors.
This road test evaluated a section of US 301 consisting of two 3.66 m (12 ft)
wide lanes with a 229-178-229 mm (9-7-9 in) thickened edge cross-section.
The pavement had been built in 1941. The slabs were reinforced with wire
mesh, and had 12.2 m (40 ft) contraction joint spacing and 36.6 m (120 ft)
expansion joint spacing (Yoder and Witczak 1975: 597).
Truck loads of 80 and 100 kN (18,000 and 22,400 lb) single axles
and 142 and 200 kN (32,000 and 44,800 lb) tandem axles were applied
between June and December 1950 (Huang 2004: 19–20). The primary aim
of this road test was not road design, but to determine proper tax allocation
between trucking and railroads.
These road tests applied accelerated traffic to pavements, simulating a
lifetime of traffic within a few months. However, it was not possible to
accelerate environmental effects in the field. Pasko (1998) notes “One also
needs to look at the effects of uncontrolled variables (environment) on
pavement performance. A good example is the Road Test One – MD where
controlled testing during July and August produced negligible damage. In
September, the area had very heavy rains. In August, eight joints were
pumping compared to 20 and 28 in September and October, respectively.
The edge pumping was 162 ft (50 m) in August, 462 ft (140 m) in September,
and 380 ft (116 m) in October after the heavy rain.”
At the Maryland Road Test, progression of cracking was definitely linked
to the development of pumping. Pumping was found to be greatest at expan-
sion joints. Pumping occurred on plastic clay soils, but not on granular
subgrades with low percentages of silt and clay. Deflections due to temper-
ature curling and warping were also measured, and found to be significant
(Yoder and Witczak 1975: 598).
The first concrete airfield pavement was built in 1928 at Ford Field in
Dearborn, Michigan. Lunken Field in Cincinnati, Ohio, was constructed
a year later. Like many early highway pavements, these airfields used a
thickened-edge section, with the pavement at the edge 50 mm (2 in) thicker
than at the centerline. Throughout the 1930s, the predominant aircraft
was the relatively light DC-3, so the trucks that delivered fuel to the air-
craft controlled the design. Early airfield concrete pavements were generally
152 mm (6 in) thick. The advent of the B-29 Superfortress bomber in World
War II required 305 mm (12 in) pavements, so existing pavements were
overlaid with 152–178 mm (6–7 in) of new concrete. With larger post-
war bombers, pavement thickness increased to 508–686 mm (20–27 in)
The work of the US Army Corps of Engineers in concrete pavement
development was significant, particularly for airfields. With the B-29 in late
World War II and progressively heavier postwar long range bombers, the
Corps faced the difficult task of designing pavements around the world
for very heavy loadings. In 1975, Yoder and Witczak noted that the
“Corps has for the past 20 years conducted extensive research programs
on prototype pavements as well as pavement test sections” (Yoder and
Witczak 1975: 4).
Ray (1981: 4–8) summarized the advances in pavement design and per-
formance that were made between 1945 and 1980.
• Based on observations of pavement deformation due to expansion or
shrinkage of highly expansive soils in the late 1930s, treatments for
these soils with cement or lime were developed.
• Mechanisms of frost heave were identified and analyzed, and meth-
ods to address frost heave through careful subgrade construction and
relatively thin granular subbase layers were adopted.
• Pumping was identified as a potential failure mechanism for concrete
pavement joints, and soils and conditions susceptible to pumping were
identified. Pumping may be controlled through use of granular subbases
and doweled joints.
• Inadequate drainage or nonuniform compaction can lead to problems
with thin granular subbases.
• Cement-treated bases (CTBs) or subbases provide excellent support and
• Under the right conditions, thin concrete pavements can provide satis-
factory service. Some 150 mm (6 in) airfield pavements lasted 30 years
or more as long as the design aircraft wheel loads were not exceeded.
Similarly, Iowa rural farm-to-market roads only 110 mm (4½ in) thick
carried traffic for 30 years.
• Even if slab stresses are not high, excessive deflections can lead to
pavement performance problems by aggravating curling and warping
• Most agencies switched exclusively to jointed plain concrete pave-
ment (JPCP) from jointed reinforced concrete pavement (JRCP) due
to spalling, blowups, and broken reinforcement at intermediate cracks
that form in JRCP slabs.
• Problems with undoweled JPCP joints led to wider adoption of dowels
for highway and airport pavements.
• JPCP with short joint spacing on the order of 4.6 m (15 ft) provides
the lowest life cycle costs for most applications.
• Concrete shoulders tied to mainline concrete pavements reduce deflec-
tions and stresses and improve safety and surface drainage and reduce
• Properly designed and built overlays – either bonded, unbonded, or
whitetopping – can provide many years of service.
The AASHO road test
The Dwight D. Eisenhower Federal-Aid Highway Act of 1956 created
the 66,000 km (41,000 mile) interstate highway system. Sixty percent
of the system was paved with concrete. There was obviously a need for
research to support this construction effort. The AASHO Road Test, a
$27-million study, was undertaken near Ottawa, Illinois. Six different test
loops were built and loaded around the clock for 2 years. Twelve dif-
ferent combinations of axles and many thicknesses of asphalt and con-
crete were evaluated in order to establish performance histories and trends
Pasko (1998) notes that
At the AASHO Road Test, there were two distinctive failure modes for
concrete pavements. The very thin pavements failed with continuous
edge pumping that caused edge-cracking that coalesced into a longitu-
dinal edge crack. The thicker pavements failed by joint pumping that
caused transverse cracking starting particularly in the traffic leave side
of the joints. The data from both were averaged together in the road
test analysis to develop a performance equation. Even so, of the 84
pavement test sections greater than 8 in (200 mm) in thickness, only
seven sections had a serviceability index of less than 4.0 at the end of
the testing. In fact, only three sections could actually be considered as
having failed. Hence, one can conclude that even though the AASHO
data is the best that we have, it hardly predicts failure of the thicknesses
of pavement that are now being built (greater than 8 in). Additionally,
at the road test, there were no punchthroughs (shear failure) such as
those produced at the Pittsburg Road Test under steel wheels, nor were
there other types of environmentally induced failures such as blow-ups,
CRCP punchouts, and so forth.
Early concrete pavements often suffered distress due to freezing and thawing
cycles, or scaling due to deicing salts, or subgrade pumping. These problems
were addressed during the 1930s, with air entrainment of concrete to attack
the durability problems. The conditions likely to lead to pumping were
identified – subgrade soil with fines that could go into suspension, water in
the subgrade, and frequent heavy axle loads. Where these conditions exist,
subbase layers between the concrete pavement and the subgrade are used
to prevent pumping.
During this period, improvements to concrete paving equipment had been
relatively minor, with motorized mixers replacing hand mixers. Pavements
were placed using relatively expensive side forms. The slipform paver was
developed in Iowa between 1946 and 1949 by two state highway engineers,
James W. Johnson and Bert Myers. The innovation was first used in 1949 to
pave a 2.7 m (9 ft) wide, 150 mm (6 in) thick county road. By using two pavers
side by side, a county road could be paved in one pass. By 1955, the Quad City
Construction Company had developed an improved, track propelled paver
that could place 7.3 m (24 ft) wide slabs 250 mm (10 in) thick, and over time
even larger pavers were developed. During this time, sawn joints began to
replace hand-tooled joints and improve pavement smoothness.
Construction practices also improved. “The 1960’s and Interstate con-
struction also saw a number of advances in concrete pavement construction
technology. Electronic controls were added to slipform pavers. Subgrade
trimmers were introduced for better grade control. Tied concrete shoulders,
first tested in Illinois in 1964, were found to add significant structural value
to concrete pavements. Concrete saws were increased in size and capability.”
(ACPA 2006). Central mixing plants increased production capacity by a
factor of 10 over the previous dry batch process. The net result of this work
was dramatic improvements in speed of construction.
Elements of modern slipform roadway paving are shown in Figures 1.1
through 1.3. In Figure 1.1, dowel and tie bars have been placed and secured
in baskets in order to provide load transfer across sawn joints. Figure 1.2
Figure 1.1 Dowel and tie bar baskets placed in preparation for slipform paving (photo
courtesy of The Great Lakes Construction Company, Hinckley, Ohio).
Figure 1.2 (a) and (b) Slipform pavers (photo courtesy of The Great Lakes Cons-
truction Company, Hinckley, Ohio).
Figure 1.3 Finishing slipformed pavement around a banked curve (photo courtesy of The
Great Lakes Construction Company, Hinckley, Ohio).
illustrates the extrusion of concrete from the slipform paver itself, along
with finishing operations. Figure 1.3 shows how slipforming can be used
around a banked curve.
Evolution of design
Yoder and Witczak note that in the early development of concrete pave-
ments, they were built directly on subgrade regardless of subgrade type or
drainage conditions. Typical slab thicknesses were 152–178 mm (6–7 in).
With increasing traffic after World War II, pumping became an increasingly
important phenomenon, although it had been described as early as 1932
(Yoder and Witczak 1975: 596).
Thickened edge sections were common in the 1930s and 1940s. For
example, a pavement would be built 152 mm (6 in) thick in the center
and 203 mm (8 in) thick along the edges, which was described as an 8-6-8
design. Pavements were typically only 5.5–6.1 m (18–20 ft) wide (Yoder
and Witczak 1975: 596–597).
As designs evolved, pavements were built over granular subbases to pre-
vent pumping. In northern climates, thick bases were also used for frost
protection. Pavement thickness was increased to 229–254 mm (9–10 in) for
highways (Yoder and Witczak 1975: 596–597). In modern practice, thicker
designs are often used for heavily traveled highways.
The long term pavement performance program
The last and greatest road test of all began in 1987 and continued for
the next two decades (and in fact continues today). This was the Federal
Highway Administration long term pavement performance (FHWA LTPP)
program, which is part of the strategic highway research program (SHRP).
The LTPP experiment encompassed rigorous field tests of more than 2,400
500 m (1,640 ft) asphalt and concrete pavement sections across the United
States and Canada (FHWA LTPP 2006).
The program consisted of both pavements that were in service at the
beginning of the test, termed general pavement studies (GPS) sections, and
pavement sections that were constructed specifically for the LTPP, termed
specific pavement studies (SPS) sections. SPS sections were constructed to
a specific experimental design within each experiment. In the original pro-
gram, there were 777 GPS sites and 234 SPS sites (Huang 2004: 26). An
additional experiment was the seasonal monitoring program (SMP) that
focused on environmental effects.
Within the GPS program, GPS-3, GPS-4, and GPS-5 analyzed JPCP,
JRCP, and continuously reinforced concrete pavement (CRCP), respectively.
Two other experiments analyzed concrete overlays on concrete pavements,
with GPS-8 for bonded overlays and GPS-9 for unbonded overlays (Huang
2004: 25–26). However, the GPS-8 bonded concrete overlay program was
Five of the nine SPS programs were relevant to rigid pavements. These
were SPS-2, structural factors, SPS-4, preventive maintenance effectiveness,
SPS-6, rehabilitation, SPS-7, bonded concrete overlays, and SPS-8, study
of environmental effects in the absence of heavy loads (Huang 2004: 26).
Because few states were willing to construct bonded concrete overlay test
sections, only four sites were built, and the SPS-7 experiment was termi-
All sites had original inventory information and materials samples col-
lected. LTPP pavement sites are visited periodically by contractors for data
collection. Data collected includes traffic, profile, smoothness, distress, fric-
tion, and falling weight deflectometer (FWD) readings. Detailed climate
information is also gathered (Huang 2004: 25–26).
The LTPP program offered many advantages over previous road tests. The
previous tests were limited to a single geographical location, and generally
used accelerated traffic loading. Accelerated traffic tends to obscure the
importance of environmental effects. In contrast, the LTPP program is
nearly two decades old, and realistic traffic and environmental conditions
have been monitored over that time.
The LTPP program produced a large number of research reports and
design and analysis tools, including the spreadsheet-based 1998 Ameri-
can Association of State Highway and Transportation Officials (AASHTO)
rigid pavement design procedure (AASHTO 1998). However, the greatest
importance of the LTPP program was in the development and calibration
of models for the new AASHTO Mechanistic-Empirical Pavement Design
In order to make LTPP data more accessible to users, the FHWA pub-
lished several versions of DataPave software. For several years, the LTPP
data and DataPave software were used for a student contest (Delatte
2002). The software has been superseded by DataPave Online, a website
that allows users to access and analyze LTPP data. “The LTPP DataPave
Online is a major effort to make the LTPP data more accessible to world-
wide transportation community” (FHWA DataPave 2006). The Trans-
portation Research Board (TRB) also has a program for LTPP studies
Economy, service life, and life cycle costs
Highway agencies have reported service lives for concrete pavements of
as much as 25–40 years, or generally 11/2–2 times the service life of
asphalt pavements designed and built to similar standards. In general,
concrete is selected for heavily trafficked pavements and typically carries
four times as much daily truck traffic as asphalt pavements. Respective
life cycle costs of pavement designs depend greatly on material costs at
the time of construction, but concrete pavements often have significantly
lower maintenance costs although initial construction costs may be higher
Challenges for the future
The interstate highway system was a monumental and historic undertaking.
However, in some respects, the engineers and builders of the early highways
and the interstate highway system had an easier task than those of today. As
the highway system has become built out, it must be maintained, repaired,
and reconstructed while, in many cases, allowing traffic to continue to
use the roadway. Much tighter environmental controls are now in place,
and quality raw materials for use in highway construction are becoming
increasingly scarce in many areas. Concrete overlays of various types have
an important part to play in the upgrading and maintaining of the overall
network. Accelerated or “fast track” paving materials and techniques have
been developed to get traffic onto pavements more quickly.
Maintenance and rehabilitation
Even the best designed and built concrete pavements will eventually wear
out and require maintenance or rehabilitation. Concrete pavement perfor-
mance and distress are addressed in Chapter 3. Maintenance techniques and
maintenance management are discussed in Chapter 16, and rehabilitation
techniques in Chapter 17. It is important to recognize that timely main-
tenance, or pavement preservation, can substantially extend pavement life
and delay the need for rehabilitation. When major work becomes necessary,
overlays, as discussed in Chapter 18, may be used.
An effective maintenance and rehabilitation program, however, also
requires a deeper understanding of how pavements behave. The basic design
aspects discussed in Chapter 7 can provide insight as to whether a partic-
ular pavement distress may be due to inadequate pavement thickness, an
unstable subbase material, or excessive joint spacing.
Meeting congestion and safety challenges
“Rehabilitation of today’s highways requires traffic management, con-
tracting and construction techniques that are quick and efficient and that
result in a pavement with superior rideability and service life” (ACPA
2000c: 1). Pavement maintenance and rehabilitation are particularly chal-
lenging for high volume pavements, particularly in congested urban areas.
The American Concrete Pavement Association (ACPA) has published Traf-
fic Management – Handbook for Concrete Pavement Reconstruction and
Rehabilitation (ACPA 2000c) to address some of these issues. Some impor-
tant points made in that document include:
• On many urban freeway reconstruction projects, the road user delay
costs may exceed $50,000 per day.
• Concrete pavement does not require a curing time of 5–14 days
before opening to traffic – mixtures are available that allow traffic in
• Limiting contractors to single lane closures or nighttime work hours
may be unwise for both safety and productivity.
• The public generally prefers a short project with major disruptions to
a long project with smaller disruptions. The slogan is “get in, get out,
• Issues that should be addressed include scope of the project, traf-
fic management, safety, construction requirements, innovative bidding,
constructability, emergency planning, and public information and coor-
• Innovative bidding and contracting practices, such as incen-
tives/disincentives and A+B bidding (bidding both price and time),
motivate and challenge contractors to finish projects and open them to
public traffic more quickly.
• Bridge abutments and clearances may constrict the range of available
work zone configuration options, and should be considered early in the
• Recycling paving materials in place, as discussed later in this chapter,
reduces project duration.
• Availability and capacity of detour routes and access for work vehicles
are key considerations. Pavements and bridges on detour routes that
will carry significant increases in traffic require structural evaluation.
• It is important to communicate with the public about the impacts,
future benefits, and progress of the project to establish and maintain
Non-destructive testing technologies such as maturity or ultrasonic pulse
velocity can estimate in-place pavement strength for opening to traffic.
ACPA (2000c: 28) provides a table for determining the strength necessary
to open the concrete pavement to public traffic.
Safety in US highway construction work zones is addressed in Part VI of
the Manual on Uniform Traffic Control Devices (FHWA 2003). Conges-
tion and capacity may be analyzed using Highway Capacity Manual 2000
Accelerated concrete pavement construction and reconstruction are also
addressed by the American Concrete Institute (ACI) committee report Accel-
erated Techniques for Concrete Paving, ACI 325.11R-01 (ACI Committee
325 2001). It is important to note that accelerated paving does not always
require high early strength concrete. With materials and mixtures in use
today, conventional paving concrete generally achieves sufficient strength
to carry traffic in 2–4 days, so if opening to traffic can be delayed that long
there is no need to use high early strength concrete. Small weekend closure
projects such as urban intersections can be built with conventional paving
concrete. If all concrete is placed by Saturday evening, it will have a day
and a half to cure for a Monday morning opening.
One interesting case study is the reconstruction of heavily trafficked
Interstate Highway 15 in Southern California. The concrete truck lanes
were badly deteriorated, and a 4.5 km (2.8 mile) section was rebuilt in
only two nine day closures. Because this is the main highway between Los
Angeles and Las Vegas, it has heavy traffic on weekends. The project is
discussed in detail by Lee et al. (2005). Some of the key features of the
• The pavement was rebuilt in nine day closures as opposed to overnight
closures, because the longer closures had been found to yield much
higher contractor productivity.
• Longer closures reduce the overall disruption to the traveling public,
provide greater life expectancy for the pavement, improve safety, and
significantly reduce construction costs.
• The existing pavement of 200 mm (8 in) of concrete over 100 mm
(4 in) of CTB over 300 mm (12 in) of aggregate base was replaced with
290 mm (11½ in) of concrete over 150 mm (6 in) of asphalt over half of
the reused aggregate base. The pavement grade was not changed. The
outer truck lane was widened by 600 mm (2 ft) to reduce edge-loading
• Caltrans went to considerable effort to communicate to the public how
the selected strategy would reduce the overall project duration and
minimize disruption to the traveling public. An automated work zone
information system gave the public travel time and detour informa-
tion on changeable message signs. Public outreach materials included
comprehensive project brochures and flyers, a construction advisory
electronic bulletin, and a project information hotline. A project website
was used to communicate information to the public and also to gather
feedback. Several public meetings were held for local communities.
• Rapid strength gain concrete with type III cement allowed opening the
pavement to traffic in 12 hours. About 50 percent of the project was
able to use a more conventional concrete with type II cement, as long
as 24 hours of curing was available.
• Project completion time incentives and disincentives and late opening
penalties were specified in the contract.
On larger projects, the bulk of the project may be paved with regular
concrete with small amounts of high early strength concrete used for small
final closure strips. This approach was adopted for critical taxiway tie-
ins during new runway construction at Cleveland Hopkins International
Airport, although it was found that with proper planning the conventional
concrete achieved sufficient early strength and it was not necessary to use
high early strength concrete (Peshkin et al. 2006b).
Case studies of similar projects can provide valuable insights into avail-
able techniques and strategies. Peshkin et al. (2006a,b) review a number of
airport case studies. The ACPA report Traffic Management – Handbook
for Concrete Pavement Reconstruction and Rehabilitation (ACPA 2000c:
iii, 50) discusses highway and street case studies:
• Reconstruction of the Eden’s Expressway in north suburban Chicago
required the Illinois DOT to use a wide range of accelerated paving
techniques and provided much of the information for the ACPA Hand-
• In Denver, Colorado, 75 days were cut from a 200-day schedule for
construction of an urban arterial.
• In Johnson County, Kansas, a major intersection was repaved over a
weekend with a whitetopping overlay.
If high early strength concrete is used, it is important to consider durability.
Some mixtures that achieve strength in 6–8 hours have shown durabil-
ity problems, although not in all cases. Durability of high early strength
concrete is discussed in Chapter 6 and by Van Dam et al. (2005). It is
particularly frustrating to agencies and users when repairs fail quickly and
need to be repeated.
Recycling and reuse of materials
The construction of highways, bridges and buildings has been increasing
from the beginning of the past century, especially in areas of high
population density. These facilities need to be repaired or replaced
with the passing of time because their end of service life is reached or
the original design no longer satisfies the needs due to the growth in
population or traffic. These facts have generated two important issues.
First, a growing demand for construction aggregates and, second, an
increase in the amount of construction waste. Two billion tons of
aggregate are produced each year in the United States. Production is
expected to increase to more than 2.5 billion tons per year by the
year 2020. This has raised concerns about the availability of natural
aggregates and where we will find new aggregate sources. On the other
hand, the construction waste produced from building demolition alone
is estimated to be 123 million tons per year. Historically, the most
common method of managing this material has been through disposal
in landfills. As cost, environmental regulations and land use policies for
landfills become more restrictive, the need to seek alternative uses of the
waste material increases. This situation has led state agencies and the
aggregate industry to begin recycling concrete debris as an alternative
(FHWA 2004: 5–6)
Pavements with steel reinforcement may also be recycled, and equipment has
been developed to economically remove reinforcement and dowels without
the need for hand labor. Continuous steel or mesh is usually removed at
the demolition site, while dowels and tie bars may be removed at a plant
where the material is processed (ACPA 1993c). Any reinforcing steel in the
concrete has to be removed.
Existing concrete can be crushed and recycled into concrete pavement,
either as new concrete pavement or as a base or subbase course under
concrete pavement. Crushing and processing may occur at or very near
to the construction site. The recycled concrete aggregate (RCA) offers a
number of advantages:
• reduces the need for virgin aggregates;
• reduces the volume of waste materials brought to landfills;
• reduces transportation costs as well as the number of trucks that must
maneuver in and out of the work zone, which can reduce project dura-
tions as well as costs;
• residual cementitious properties as well as the angularity of crushed
concrete particles can enhance the stability and stiffness of a recycled
concrete base or subbase;
• when old concrete is crushed to a smaller size, susceptibility to D-
cracking is reduced.
There are also some risks and cautions associated with the re-use of existing
• Existing concrete often has unknown properties. Construction debris
may contain unwanted bricks, wood, steel, ceramics, glass, or other
materials. As a result, some agencies only allow concrete from their
previous agency or DOT projects to be recycled for their new projects.
• Use of RCA in new concrete can create workability problems unless
the moisture content of the material is controlled.
• Some RCA needs to be washed before being used in new concrete,
which adds to cost.
• Fines in unwashed RCA may reduce concrete compressive strength.
• RCA generally has a higher absorption and lower specific gravity than
the original aggregate used in the concrete, due to the inclusion of
mortar made of cement, water, and air. It is best to keep stockpiles in
saturated surface dry (SSD) condition.
• When used as a base or subbase, the RCA should be kept wet to limit
dust and excess working should be avoided to prevent segregation. The
material should be compacted in a saturated condition.
• Concerns about leaching remain when RCA is used in a drainage layer
or near a water source.
The Federal Highway Administration Recycling Team performed a national
review of the state of the practice in Transportation Applications of Recy-
cled Concrete Aggregate. The study identified 41 states recycling concrete
aggregate, with 38 using it as aggregate base and 11 as an aggregate for PCC.
The report reviewed and summarized state practices in Texas, Virginia,
Michigan, Minnesota and California. Texas, Minnesota, and California
reported that RCA performed better than virgin aggregate as a base. One
value engineering proposal in Michigan saved $114,000 on a $3 million
project through use of RCA. Michigan has also used recycled concrete
as backfill for edge-drains. Two developments that make the use of RCA
more attractive are the use of mobile crusher units that can be moved to
stockpiles of construction debris, and mobile units that crush pavement in
place into base or subbase material (FHWA 2004). The FHWA has estab-
lished a website at http://www.fhwa.dot.gov/pavement/recycling/index.cfm
to provide information on recycling.
An important thing to remember is that concrete often fails for a reason.
If the concrete failed due to fatigue, there is little risk involved in recycling
the material. On the other hand, if the failure was due to a material-related
distress such as alkali-silica reaction (ASR), recycling the material into new
concrete simply sets the stage for a future failure. One cautionary tale
on the problems that can occur when crushed concrete is recycled in an
environment prone to sulfate attack is discussed in detail by Rollings et al.
(2006) and reviewed briefly in Chapter 5. It may be prudent to carefully
examine the existing concrete for ASR or D-cracking problems to determine
whether recycling is an option (ACPA 1993c).
When the concrete pavement has a thin asphalt overlay, it is possible
to crush the two together if it is to be used as a base or a subbase, but
not in new concrete. The asphalt in the material is not harmful, and it is
not necessary to mill off the overlay. Minnesota allows up to 3 percent
asphalt cement or approximately 50 percent reclaimed asphalt pavement
(RAP) in the crushed base material. California goes further and allows any
combination of RCA and RAP (FHWA 2004: 26).
The ACPA has published Recycling Concrete Pavement, Technical Bul-
letin TB–014.P, which discusses concrete pavement recycling from old pave-
ment removal, to concrete crushing, to replacing the new pavement. The
bulletin covers critical aspects of mix design for RCA in fresh concrete. It
may be necessary to determine the optimum rate of recycled concrete fines
in the mixture, and to pay special attention to control of water content.
A guide specification is included in the Bulletin (ACPA 1993c).
Road and airport construction and the production of concrete and other
construction materials have environmental impacts. For the most part, the
impacts of development on the landscape are similar regardless of the pave-
ment type, with the exception of pervious pavements. Also, both asphalt and
concrete pavements require large quantities of aggregate, so their impact
through aggregate mining and production are similar.
The production of portland cement impacts the environment due to the
large amounts of energy required and the release of CO2 into the atmo-
sphere. Concrete production requires approximately 3.4 GJ per cubic meter
(Mindess et al. 2003: 5). “As a major part of the world economy, the con-
crete industry must play an active role in sustainable development. Because
there are few new technologies on the horizon that can reduce CO2 emis-
sions from the manufacturing of portland cement, however, the answer to
reducing CO2 emissions lies in minimizing the output of cement clinker”
(Malhotra 2006: 42).
The total worldwide annual production of fly ash is about 900 million
tonnes (990 million tons), principally in China, India, and the US. China
alone produces two-thirds of the worldwide amount. Use of coal in power
plants, and therefore production of fly ash, is expected to increase substan-
tially in these countries over the next few decades. These countries currently
use approximately 10–15 percent of the fly ash in concrete. In the United
States, fly ash is separately batched at concrete plants, whereas overseas
the fly ash is often blended into the cement at a rate of about 20 percent
(Malhotra 2006: 42–43).
Not all fly ash meets specifications for use in concrete. Most of the fly
ash that does is type F, which is a by-product of combustion of anthracite
or bituminous coal, and has pozzolanic but not cementitious properties.
High calcium fly ash, type C, which has cementitious properties as well
as pozzolanic properties, is produced from lignite or sub-bituminous coal.
“Technologies are available, however, that can beneficiate fly ash that fails
to meet fineness and carbon content requirements – the two most important
parameters of fly ash used in concrete. These technologies include removal
of carbon by electrostatic and floatation methods. Grinding and air classifi-
cation methods have also been used to produce fly ash with high fineness”
(Malhotra 2006: 43).
Malhotra (2006: 45) suggests reducing CO2 emissions using the following
• “Using less portland cement;
• Using more supplementary cementitious materials;
• Using less unit water content by using more water-reducing admixtures
and HRWRAs [high-range water reducing admixtures];
• Incorporating recycled aggregates in concrete;
• Where possible, specifying strength acceptance criteria at 56 or 91 days
instead of 28 days.”
For paving concrete, then, the strategies for reducing cement use and thus
CO2 emissions are:
• maximize the aggregate structure as discussed in Chapter 6 to minimize
the overall paste volume;
• use water reducers to reduce the amount of water and thus the cementi-
tious material content required to maintain the same water/cementitious
materials (w/cm) ratio; and
• replace as much cement as practicable with fly ash or ground granulate
blast furnace slag (GGBFS).
Malhotra (2006: 43–44) has developed high volume fly ash (HVFA) con-
crete where as much as half or more of the cement is replaced by fly ash.
To date, HVFA concrete has not been used for pavement, to the author’s
Some other supplementary cementitious materials that could be used in
paving concrete are GGBFS, natural pozzolans, rice-husk ash, silica fume,
and metakaolin. GGBFS is already extensively used in paving concrete,
but availability is limited. Only about 25 million tonnes (28 million tons)
are produced a year. Rice-husk ash is not yet commercially available, but
the estimated worldwide potential is 20 million tonnes (22 million tons).
Silica fume and metakaolin are only available worldwide in relatively small
quantities (Malhotra 2006: 44). To date, silica fume and metakaolin have
not been widely used for pavements. Silica fume has been used for dense
concrete bridge deck overlays, and could be used for pavement bonded
Sustainable development is of increasing interest, and was written into
the American Society of Civil Engineers Code of Ethics in 1996. This
was added as item 1e – “Engineers should seek opportunities to be of
constructive service in civic affairs and work for the advancement of
the safety, health and well-being of their communities, and the protec-
tion of the environment through the practice of sustainable development”
Sustainable development is defined as “the challenge of meeting human
needs for natural resources, industrial products, energy, food, transporta-
tion, shelter, and effective waste management while conserving and protect-
ing environmental quality and the natural resource base essential for future
development” (ASCE 2006). Another term for sustainable development is
Pavements represent an important potential application area for sus-
tainability concepts. “As the world’s non-renewable resources such as fos-
sil fuels and roadway aggregates decrease in availability, it is important
for all levels of government to begin considering paving structures on a
sustainability basis rather than just a first cost basis” (Smith and Jolly
Some of the environmental and sustainability benefits of concrete pave-
• Reductions of 2.4–30 percent in energy requirements for pavement
construction and maintenance, with higher savings for more heavily
• Reduced heavy vehicle fuel consumption and greenhouse gas produc-
tion (particularly CO2) because concrete pavement has less rolling resis-
tance, therefore requiring lower vehicle power. Fuel reductions of up
to 20 percent have been observed.
• Concrete pavements use less granular material or aggregate throughout
the pavement structure because base layers are not needed. Asphalt
pavements may use twice as much. These materials are growing scarcer,
and hauling aggregates represents a significant fraction of the environ-
mental impact of highway construction.
• Supplementary cementitious materials – fly ash, ground granulated blast
furnace slag, and silica fume – are industrial by-products and their use
in concrete reduces volumes of waste.
• Concrete pavements reduce the heat island effect. Urban areas tend to
be 5 C 9 F warmer than the surrounding countryside because dark
pavements and roofs retain heat. Concrete pavement has a lighter color
and reflects light, reducing the heat island effect. Black surfaces can be
21 C 38 F warmer than the most reflective white surfaces. Reducing
the heat island effect can also reduce smog and ozone in urban areas.
• Because concrete is more reflective than asphalt, lighting requirements
are lower for concrete parking lots, reducing energy consumption
(Smith and Jolly 2005: 585–606).
An US Environmental Protection Agency (EPA) website on the heat island
effect states “For millions of Americans living in and around cities, heat
islands are of growing concern. This phenomenon describes urban and sub-
urban temperatures that are 2 to 10 F (1 to 6 C) hotter than nearby rural
areas. Elevated temperatures can impact communities by increasing peak
energy demand, air conditioning costs, air pollution levels, and heat-related
illness and mortality” (EPA 2006). Lighter colored and porous paving mate-
rials are recommended by the EPA for reducing the heat island effect.
One way of addressing sustainability in constructed facilities is through
the leadership in energy and environmental design (LEED) program.
Although LEED primarily applies to buildings, it provides principles that
are relevant to sustainability in general, and applies to parking facilities
and industrial pavements. Under LEED, buildings are eligible for points
that may be used to achieve different levels of certification. Potential LEED
points applicable to ready-mixed concrete include storm water manage-
ment, landscape paving, managing construction waste, use of recycled
materials, and reductions in the use of portland cement (RMC Research
Possible LEED strategies include:
• use of pervious concrete pavement, discussed in Chapter 2;
• concrete parking lots to reduce the heat island effect;
• diversion of construction debris from landfills through recycling or
salvage, which primarily applies to overlays, discussed in Chapter 18;
• use of by-products as supplementary cementitious materials, such as
fly ash, GGBFS, silica fume, or rice-husk ash. Use of these materials in
concrete usually reduces the amount of portland cement needed;
• use of local materials to reduce transportation costs (RMC Research
The Environmental Council of Concrete Organizations (ECCO) (www.
As a nearly inert material, concrete is an ideal medium for recycling
waste or industrial byproducts. Many materials that would end up in
landfills can be used instead to make concrete. Blast furnace slag, recy-
cled polystyrene, and fly ash are among materials that can be included
in the recipe for concrete and further enhance its appeal. Waste prod-
ucts such as scrap tires and kiln dust are used to fuel the manufacture
of cement. And even old concrete itself can be reborn as aggregate for
new concrete mixtures.
Another environmental plus for concrete is energy efficiency. From
manufacture to transport to construction, concrete is modest in its
energy needs and generous in its payback. The only energy intensive
demand is in the manufacture of portland cement, typically a 10–15%
component of concrete. Since the materials for concrete are so readily
available, concrete products and ready-mixed concrete can be made
from local resources and processed near a jobsite. Local shipping min-
imizes fuel requirements for handling and transportation.
Sources for information, research reports,
guidelines, and standards
A number of organizations publish references that are useful to the concrete
pavement engineer. Many of these references were consulted during the
development of this book and are listed in the bibliography. Although many
of these organizations are in the United States, their documents are often
used and referenced worldwide.
The websites will be useful to readers who would like to pursue the topics
discussed. Also, readers who wish to keep up with the latest developments
or contribute to the state of the practice may wish to participate in one or
more of these organizations.
One of the oldest organizations to develop information for concrete pave-
ments is the Portland Cement Association (PCA), website www.cement.org.
The PCA developed a number of important pavement design guides
up through the 1980s. The American Concrete Pavement Association
(ACPA), website www.pavement.com, subsequently has assumed most
of the PCA’s concrete pavement work. At present, the ACPA publishes
design and construction documents for highways, parking lots, streets
and local roads, airports, and industrial pavements. The ACPA and PCA
also sell a number of concrete pavement design computer programs.
The PCA continues to publish literature on roller-compacted concrete
(RCC) pavements as well as cement-stabilized base and subbase layers, as
well as a key publication on Design and Control of Concrete Mixtures
(Kosmatka et al. 2002).
The National Ready Mixed Concrete Association (NRMCA), website
http://www.nrmca.org/, is at present the primary source for information on
pervious concrete pavements. NRMCA also provides a number of certifica-
tions for concrete suppliers and contractors. The PCA, ACPA, NRMCA are
all industry associations that are supported and financed by their members.
All three of these organizations employ engineers to draft their technical
documents and also contract for outside research.
The American Concrete Institute (ACI), website www.concrete.org,
works to advance concrete knowledge through a large number of techni-
cal committees. The four technical committees most directly relevant to
concrete pavement are 325 Concrete Pavements, 327 Roller Compacted
Concrete Pavements, 330 Concrete Parking Lots and Site Paving, and 522
Pervious Concrete. The technical committee membership includes members
of industry associations, government agency representatives (e.g. FHWA,
FAA, and USACE, discussed below), academics, and consulting engineers.
Documents are produced through a rigorous consensus process, which
means they take longer to develop but are often more authoritative than
those from other sources. The documents of the four pavement committees,
as well as many others with direct application to pavements (e.g. mix-
ture proportioning, testing, and curing), are contained in the six volume
Manual of Concrete Practice and may also be purchased separately. ACI
also has a number of certification programs for testing laboratories and
ACI, APCA, and PCA publications are particularly relevant for concrete
pavement types that are not addressed by governmental organizations such
as FHWA, AASHTO, or PCA. These include parking lots, streets and local
roads, RCC, pervious concrete, and industrial pavements.
The American Society for Testing and Materials (ASTM), website
www.astm.org, works through technical committees in a similar manner to
ACI. There is also some overlap of membership between the two organiza-
tions. ASTM publishes testing protocols and materials standards.
The Transportation Research Board (TRB) is a division of the National
Research Council. The TRB website is www.trb.org. The National Research
Council is jointly administered by the National Academy of Sciences, the
National Academy of Engineering, and the Institute of Medicine. TRB is a
very large organization with international membership that covers a broad
array of transportation topics, including concrete and concrete pavement.
Concrete pavement research results are often presented at the TRB annual
meeting, and papers are published in Transportation Research Record
(TRB). Like ACI and ASTM, TRB works through constituent committees.
TRB was formerly the Highway Research Board.
The International Society for Concrete Pavements (ISCP), website
http://www.concretepavements.org/, is a relatively young organization
whose main activity has been to organize the International Conferences
on Concrete Pavements. Eight of these conferences have been held every 4
years, and the conference proceedings are a valuable source of information.
Many ISCP members also participate in TRB and ACI.
Under the United States Department of Transportation, the Federal
Highways Administration (FHWA), website http://www.fhwa.dot.gov/, is
responsible for highways. FHWA pavement research reports may be down-
loaded free from http://www.fhwa.dot.gov/pavement/pub_listing.cfm. The
FHWA also has a computer program for pavement drainage design, which
may also be downloaded free and is discussed in detail in Chapter 4.
The American Association of State Highway and Transportation Officials
(AASHTO), website http://www.transportation.org/, sells pavement design
guides and materials and test standards. AASHTO standards are often sim-
ilar or identical to ASTM standards. Many AASHTO documents, including
the pavement design guides, are developed under contract research through
the National Cooperative Highway Research Program (NCHRP), which
is under TRB. NCHRP online publications may be downloaded free from
Many US state Departments of Transportation have websites with
research reports and standards. There are obviously too many to list here.
In the United States, civil aviation is governed by the Federal Aviation
Administration (FAA), website http://www.faa.gov/. The FAA’s design and
construction standards are published in the Series 150 Advisory Circulars
and may be downloaded free from http://www.faa.gov/airports_airtraffic/
airports/resources/ recent_advisory_circulars/. The FAA also has free design
computer programs that may be downloaded. These are discussed in
The Innovative Pavement Research Foundation (IPRF), website
www.iprf.org, has published a number of research reports on airfield pave-
ments. IPRF reports may be downloaded free from the website.
For US military facilities, standards and guidelines are developed by
the US Army Corps of Engineers (USACE) and published as unified
facilities criteria (UFC) documents on the web at http://220.127.116.11/
report/doc_ufc.html. These include UFC 3-250-02 (2001a) “Standard Prac-
tice Manual for Rigid Pavements,” and UFC 3-260-02 (2001b) “Pavement
Design for Airfields.”
Types of concrete pavements
There are a number of different types of concrete pavements that have been
built. However, for the most part, they have two features in common. First,
they resist traffic loads through flexure of the concrete. If reinforcement is
used, it is used for crack control and not to carry load. The second element
is that concrete pavements contract due to drying shrinkage of the concrete,
and expand and contract due to thermal effects, and these movements must
be dealt with. Different types of pavements use joints, reinforcing steel,
The term “conventional concrete pavements” is generally taken to mean
either jointed plain, jointed reinforced, or continuously reinforced concrete
pavements (the first three categories described below) but not other types.
Design and detailing of joints is important for these pavements. All three
conventional pavement types have been used as overlays, although jointed
plain overlays are most common.
Prestressed and precast concrete pavements are used for similar applica-
tions as conventional concrete pavements, but have been used infrequently.
Other types of concrete pavement include roller compacted concrete (RCC)
and pervious or porous concrete, which are generally used for specialized
industrial or parking lot applications.
Jointed plain concrete pavement
Jointed plain concrete pavement, or JPCP, consists of unreinforced con-
crete slabs 3.6–6.0 m (12–20 ft) in length with transverse contraction joints
between the slabs. The joints are spaced closely enough together so that
cracks should not form in the slabs until late in the life of the pave-
ment. Therefore, for JPCP, the pavement expansions and contractions are
addressed through joints. JPCP is illustrated in Figure 2.1.
One important performance issue with JPCP is load transfer across the
joints. If joints become faulted, then drivers encounter bumps at the joints
and experience a rough ride. Two methods are used to provide load transfer
across JPCP joints – aggregate interlock and dowels.
26 Types of concrete pavements
Subbase or base
or rideability Thickness design
Figure 2.1 Jointed plain concrete pavement (JPCP) (courtesy: ACPA).
Aggregate interlock joints are formed during construction by sawing
1/4−1/3 of the way through the pavement to create a plane of weakness. A
crack then propagates through the remaining thickness of the pavement as
the concrete contracts. This crack has a rough surface because it propagates
around the aggregates through the green cement paste, and as long as
it remains narrow the joint can transfer load from one slab to another
through bearing stress of the aggregate particles against each other across
the crack. Load transfer is compromised if the joint opens too widely or if
the aggregates wear away. The quality and erosion resistance of the material
supporting the slab at the joint also affect load transfer.
Types of concrete pavements 27
When the pavement carries heavy vehicle traffic, particularly at high
speeds, aggregate interlock will break down over time and will not prevent
faulting over the life of the pavement. In this case, dowels are provided
across the joint for load transfer. Dowels are smooth rods, generally plain-
or epoxy-coated steel, which are usually greased or oiled on side to allow
the joints to open and close without resistance.
JPCP is the most commonly used type of concrete pavement because it is
usually the cheapest to construct. A 1999 survey by the American Concrete
Pavement Association identified 38 US states as constructing JPCP (ACPA
1999c). It is economical because there is no need to pay for any reinforcing
steel in the slabs or for labor to place the steel. In most regions, also, contrac-
tors will have more familiarity with JPCP than with other types of concrete
pavement. In those regions where corrosion of steel is a problem, the absence
of steel reinforcement means an absence of steel corrosion issues, although
the steel dowels can still corrode. To address dowel corrosion, a variety of
different dowel materials and coatings have been investigated (Snyder 2005).
JPC pavements, like other conventional concrete pavements, often use tie
bars to connect adjacent traffic lanes. Tie bars are deformed reinforcing steel
and, unlike dowels, are not intended to allow the joints to open and close.
Tie bars are used to separate lanes for highway pavements. In contrast,
airfield JPC pavements generally use dowels at all joints.
Most of this book’s design and construction guidelines primarily address
JPCP because it is the predominant concrete pavement type by far. Special
considerations for transitions between pavements and bridges and CRCP
details are discussed in Chapter 12.
Key performance issues of JPCP include:
• initial pavement smoothness, which is a function of construction
• adequate pavement thickness to prevent mid-slab cracking;
• limiting the joint spacing, also to prevent mid-slab cracking; and
• adequate joint design, detailing, and construction.
Jointed reinforced concrete pavement
Jointed reinforced concrete pavement, or JRCP, is distinguished from JPCP
by longer slabs and light reinforcement in the slabs. This light reinforcement
is often termed temperature steel. JRCP slab lengths typically range from
7.5 to 9 m (25–30 ft), although slab lengths up to 30 m (100 ft) have been
used. With these slab lengths, the joints must be doweled. The slab steel
content is typically in the range of 0.10–0.25 percent of the cross-sectional
area, in the longitudinal direction, with less steel in the transverse direction.
Either individual reinforcing bars or wire fabrics and meshes may be used.
Because the steel is placed at the neutral axis or midpoint of the slab, it
28 Types of concrete pavements
Figure 2.2 Jointed reinforced concrete pavement (JRCP) (courtesy: ACPA).
has no effect on the flexural performance of the concrete and serves only
to keep cracks together. JRCP is illustrated in Figure 2.2.
Although JRCP was widely used in the past, it is less common today.
The only advantage that JRCP has over JPCP is fewer joints, and this is
outweighed by the cost of the steel and the poor performance of the joints
and the cracks. Because the joints are spaced further apart than JPCP, they
open and close more, and load transfer suffers as joints open wider. JRCP
joints always use dowels. Furthermore, even though the slabs are longer,
the cracks still form at the same interval as JPCP, and therefore JRCP slabs
generally have one or two interior cracks each. The light steel reinforcement
across these cracks is generally not enough to maintain load transfer, and
therefore the cracks fault as well as the joints. As a result, the latest proposed
AASHTO M-EPDG procedure does not have provisions for JRCP. A 1999
survey by the American Concrete Pavement Association identified only nine
US states as constructing JRCP, and several of those are states that have
small highway networks (ACPA 1999c).
Continuously reinforced concrete pavement
Continuously reinforced concrete pavement, or CRCP, is characterized by
heavy steel reinforcement and an absence of joints. Much more steel is used
for CRCP than for JRCP, typically on the order of 0.4–0.8 percent by volume
in the longitudinal direction. Steel in the transverse direction is provided in a
lower percentage as temperature steel. CRCP is illustrated in Figure 2.3.
Cracks form in CRCP approximately 0.6–2 m (2–6 ft) apart. The rein-
forcement holds the cracks tightly together and provides for aggregate
interlock and shear transfer. CRC pavements require anchors at the begin-
ning and end of the pavement to keep the ends from contracting due to
shrinkage, and to help the desired crack pattern develop. Special CRCP
Types of concrete pavements 29
Figure 2.3 Continuously reinforced concrete pavement (CRCP) (courtesy: ACPA).
design considerations, including determination of the proper reinforcement
percentage, are discussed in Chapter 12.
Use of CRCP dates back to the 1921 Columbia Pike experimental road
in Virginia, with over 22,500 km (14,000 miles) of two-lane highway built
in the United States by 1982. CRCP has also been used for major airports
around the world (CRSI 1983: 1).
Because of the steel reinforcement, CRCP costs more than JRCP, and is
thus used less frequently in most regions. However, it provides a smoother
ride and a longer life than any other type of pavement, and is therefore a
preferred type in Texas and Illinois. A 1999 survey by the American Con-
crete Pavement Association identified only eight US states as constructing
CRCP (ACPA 1999c).
In many regions, the performance of CRCP has been excellent. A 2000
study of concrete pavement performance in the Southeastern US used the
LTPP database to investigate 14 CRCP sections in the states of Alabama,
Florida, Georgia, Mississippi, North Carolina, and South Carolina. At
the time of the study the sections were 21–30 years old and had carried
heavy traffic, but were generally in very good to excellent condition. With
three exceptions, the pavements had serviceability indices of 4 or better,
despite the fact that they had already exceeded their 20-year design lives
(Delatte et al. 2000: 4-3–4-6).
Key performance considerations for CRCP include:
• initial pavement smoothness;
• adequate pavement thickness to prevent excessive transverse cracking;
• adequate reinforcing steel to hold cracks together and prevent pun-
chouts. Punchouts are a distress mechanism distinct to CRCP and are
discussed in Chapter 3.
30 Types of concrete pavements
Conventional pavement joints
Conventional pavements (JPCP, JRCP, and CRCP) make use of several
types of transverse and longitudinal joints. Transverse contraction joints
are used in JPCP and JRCP, usually with dowels. At the end of each daily
paving operation, or for a significant delay in paving, transverse construc-
tion joints are placed, generally at the location of a planned contraction
joint for JPCP or JRCP. Transverse expansion or isolation joints are placed
where expansion of the pavement would damage adjacent bridges or other
drainage structures. Longitudinal contraction joints are created where two
or more lane widths or shoulders are paved at the same time. In contrast,
longitudinal construction joints are used between lanes or shoulders paved
at different times (ACPA 1996a: VII-9–VII-10).
The performance of concrete pavements depends to a large extent upon
the satisfactory performance of the joints. Most jointed concrete pave-
ment failures can be attributed to failures at the joint, as opposed to
inadequate structural capacity. Distresses that may result from joint
failure include faulting, pumping, spalling, corner breaks, blowups, and
mid-panel cracking. Characteristics that contribute to satisfactory joint
performance, such as adequate load transfer and proper concrete con-
solidation, have been identified through research and field experience.
The incorporation of these characteristics into the design, construction,
and maintenance of concrete pavements should result in joints capable
of performing satisfactorily over the life of the pavement. Regardless
of the joint sealant material used, periodic resealing will be required
to ensure satisfactory joint performance throughout the life of the
pavement. Satisfactory joint performance also depends on appropriate
pavement design standards, quality construction materials, and good
construction and maintenance procedures.
Transverse contraction joints
A transverse construction joint is defined as “a sawed, formed, or tooled
groove in a concrete slab that creates a weakened vertical plane. It reg-
ulates the location of the cracking caused by dimensional changes in the
slab, and is by far the most common type of joint in concrete pavements”
Lightly loaded jointed pavement contraction joints may rely only on
aggregate interlock across joints. More heavily loaded pavements almost
always use load transfer dowels in the joints. Dowels prevent vertical
movement or faulting between slabs, but allow the joint to open and
close to relieve stress buildup due to moisture and temperature changes in
the concrete pavement. A dowel basket assembly with corrosion resistant
Types of concrete pavements 31
Figure 2.4 Dowel basket assembly with corrosion resistant epoxy-coated dowels (photo
epoxy-coated dowels is shown in Figure 2.4. Dowel baskets are also shown
in Figure 1.1.
For jointed highways, transverse joints (usually doweled) are used perpen-
dicular to traffic, and longitudinal joints are used parallel to traffic, between
traffic lanes. Airport pavements are much wider, and jointed airport pave-
ments often use square or nearly square panels with dowels around all four
sides. Figure 2.5 shows a cross-section view of a doweled transverse joint.
The primary purpose of transverse contraction joints is to control the
cracking that results from the tensile and bending stresses in concrete
slabs caused by the cement hydration process, traffic loadings, and the
environment. Because these joints are so numerous, their performance
significantly impacts pavement performance. A distressed joint typically
exhibits faulting and/or spalling. Poor joint performance frequently
leads to further distresses such as corner breaks, blowups, and mid-
panel cracks. Such cracks may themselves begin to function as joints and
develop similar distresses. The performance of transverse contraction
joints is related to three major factors: joint spacing, load transfer across
the joint, and joint shape and sealant properties.
32 Types of concrete pavements
T/2 ± d/2
Paint and oil one end of dowel
Sealant material 1/4" – 3/8"
(6–10 mm) below surface
1 1/4" (32 mm)
T/4 ± 1/4"
Rod backup material
Figure 2.5 Doweled joint (FAA 2004: 86, 86–1).
Pavement distresses, including joint distresses, are discussed in Chapter 3.
Joint spacing and load transfer are discussed in Chapter 7, and joint shape
and sealants are discussed in Chapter 15.
A longitudinal joint is defined as
a joint between two slabs which allows slab warping without apprecia-
ble separation or cracking of the slabs Longitudinal joints are used
to relieve warping stresses and are generally needed when slab widths
exceed [4.6 m] 15 feet. Widths up to and including [4.6 m] 15 feet
have performed satisfactorily without a longitudinal joint, although
there is the possibility of some longitudinal cracking. Longitudinal
joints should coincide with pavement lane lines whenever possible, to
improve traffic operations. The paint stripe on widened lanes should be
at [3.7 m] 12 feet and the use of a rumble strip on the widened section
Types of concrete pavements 33
is recommended Load transfer at longitudinal joints is achieved
through aggregate interlock.
To aid load transfer, tie bars are often used across longitudinal joints. Tie
bars are thinner than dowels, and use deformed reinforcing bars rather than
smooth dowel bars. Design of longitudinal joints and tie bars is discussed
in Chapter 7. Tie bars in basket assemblies between lanes are shown in
Figures 1.1 and 2.6, along with dowel baskets. The tie bars are longer
and thinner than the dowel bars, and are also epoxy coated for corrosion
protection. Figure 2.7 shows a cross-section view of a longitudinal joint
with tie bars.
Longitudinal joints may be sawn or built as construction joints. If they
are sawn, basket assemblies as shown in Figures 1.1 and 2.6 are used and
the joint is sawn in a manner similar to transverse contraction joints. If
built as construction joints, tie bars are used to connect the new and old
For crowned pavements, it is important to provide a properly detailed
longitudinal joint at the crown. Otherwise, a crack is almost certain to form
there (Rollings 2001, 2005).
Figure 2.6 Tie bar basket assemblies with corrosion resistant epoxy-coated tie bars –
dowel baskets are also shown (photo by author).
34 Types of concrete pavements
T/2 ± d/2
Tie bar 30" (76 cm) Long on 30" (76 cm) Centers
Figure 2.7 Longitudinal joint (FAA 2004).
A construction joint is defined as “a joint between slabs that results when
concrete is placed at different times. This type of joint can be further broken
down into transverse and longitudinal joints” (FHWA 1990a). A header and
dowel basket for a transverse construction joint are shown in Figure 2.8.
After paving up to the header, the header will be removed. The next
paving day will start with the new concrete butted up against the old
Figure 2.8 Header and dowel basket for a transverse construction joint (photo by author).
Types of concrete pavements 35
Transverse construction joints should normally replace a planned con-
traction joint. However, they should not be skewed, as satisfactory
concrete placement and consolidation are difficult to obtain. Transverse
construction joints should be doweled and butted, as opposed to
keyed. Keyed transverse joints tend to spall and are not recommended.
It is recommended that transverse construction joints be sawed and
sealed. The reservoir dimensions should be the same as those used for
the transverse contraction joints.
Longitudinal construction joints with tie bars are discussed below.
It is essential that the tiebars be firmly anchored in the concrete. Tiebars
should be either mechanically inserted into the plastic concrete or
installed as a two-part threaded tiebar and splice coupler system. It is
recommended that periodic pullout tests be conducted to ensure the
tiebars are securely anchored in the concrete Bending of tiebars is
not encouraged. Where bending of the tiebars would be necessary, it is
recommended that a two-part threaded tiebar and splice coupler system
be used in lieu of tiebars. If tiebars must be bent and later straight-
ened during construction, Grade 40 [less than 276 MPa or 40 ksi yield
strength] steel should be used, as it better tolerates the bending. It may
be necessary to reapply a corrosion-resistant coating to the tiebars after
they have been straightened. When pullout tests are performed, they
should be conducted after the tiebars have been straightened. It is rec-
ommended that longitudinal construction joints be sawed and sealed.
The reservoir dimensions should be the same as those used for the
Keyed longitudinal joints have been used in the past but are now less
common. These joints use a sort of tongue and groove configuration where
one slab has a formed slot and the adjacent slab has a key that fits in the
slot to transfer shear. “The decision to use keyed longitudinal construction
joints should be given careful consideration. The top of the slab above the
keyway frequently fails in shear. For this reason, it is recommended that
keyways not be used when the pavement thickness is less than [250 mm]
10 inches. In these cases, the tiebars should be designed to carry the load
transfer” (FHWA 1990a).
An expansion joint is defined as “a joint placed at a specific location
to allow the pavement to expand without damaging adjacent structures
36 Types of concrete pavements
or the pavement itself” (FHWA 1990a). These are generally needed at
bridge abutments and at embedded utility structures in streets. For example,
Figure 2.4 shows a utility structure blockout adjacent to a dowel basket.
The embedded utility structure will require expansion joints.
Early pavement designs used transverse expansion joints as well as con-
traction joints, but performance was poor. One early design combined
expansion joints at 28 m (90 ft) intervals supplemented with contraction
joints at 9 m (30 ft) intervals in between. The expansion joints closed and
allowed the contraction joints to open too widely (Ray 1981: 6).
Good design and maintenance of contraction joints have virtually elim-
inated the need for expansion joints, except at fixed objects such as
structures. When expansion joints are used, the pavement moves to
close the unrestrained expansion joint over a period of a few years.
As this happens, several of the adjoining contraction joints may open,
effectively destroying their seals and aggregate interlock. The width
of an expansion joint is typically [19 mm] 3/4 inch or more. Filler
material is commonly placed [19 to 25 mm] 3/4 to 1 inch below
the slab surface to allow space for sealing material. Smooth dowels
are the most widely used method of transferring load across expan-
sion joints. Expansion joint dowels are specially fabricated with a
cap on one end of each dowel that creates a void in the slab to
accommodate the dowel as the adjacent slab closes the expansion
This detail is shown in Figure 2.9.
At bridges, expansion joints are very important, because an expand-
ing pavement can build up considerable force and damage bridge super-
structures and abutments. Expansion joints at bridges are discussed in
Joint filler materialJoint sealant material
Figure 2.9 Expansion joint detail (FHWA 1990a).
Types of concrete pavements 37
Pressure relief joints are intended to serve the same purpose as expansion
joints, except that they are installed after initial construction to relieve
pressure against structures and to alleviate potential pavement blowups.
Pressure relief joints are not recommended for routine installations.
However, they may be appropriate to relieve imminent structure damage
or under conditions where excessive compressive stresses exist.
Concrete pavements may also be used as overlays for either existing asphalt
or concrete pavements. For each of the two existing pavement types, there
are two overlay classifications based on whether the overlay is bonded to
the existing pavement, or whether the bond is either ignored or prevented,
and thus not considered in the design. A complete discussion of concrete
overlays is provided by Smith et al. (2002) and ACI Committee report
ACI 325.13R-06, Concrete Overlays for Pavement Rehabilitation (ACI
Committee 325 2006). Overlays are discussed in detail in Chapter 18.
The oldest type of concrete overlay over an existing asphalt pavement
is termed whitetopping. Generally, no special measures are taken to either
achieve or prevent bond between the new concrete and the old asphalt.
Many of these were constructed in the United States when existing asphalt
highways were added to the Interstate Highway system and upgraded. For
all practical purposes, these are designed and built as conventional concrete
pavements, using the existing asphalt as a high quality base. Special details
may be needed when the new concrete must be wider than the existing
asphalt. Traditionally, whitetopping overlay designs do not consider any
reduction in flexural stress in concrete due to bond.
However, for some time it has been recognized that the concrete bonds
to asphalt, and thinner overlays have been developed to take advantage
of that fact. Ultra-thin whitetopping (UTW) was developed in the United
States in the early 1990s, with overlays between 50 and 100 mm (2 and
4 in) in thickness. In order to reduce curling stresses in such thin pavements,
they are typically cut into squares 0.6–2 m (2–6 ft) on a side. Conventional
whitetopping overlays are typically at least 200 mm (8 in) thick.
Subsequently, thin whitetopping overlays have been developed to fill the
gap between light traffic UTW and conventional whitetopping. These are
generally 100–200 mm (4–8 in) thick, with 1.2–2 m (4–6 ft) squares. As with
UTW, thin whitetopping overlays rely on bond to reduce the flexural stress
in the concrete. A complete discussion of thin and ultrathin whitetopping
is provided by Rasmussen and Rozycki (2004).
Unbonded concrete overlays are constructed over existing concrete pave-
ments with specific measures taken to prevent bonding between the two
layers. Most commonly, the bond breaker is a thin layer of hot-mix asphalt.
The reason for the bond breaker is to keep cracks and other damage in the
38 Types of concrete pavements
existing pavement from propagating up through the new pavement – this
propagation is termed “reflective cracking.” With the bond breaker layer,
the existing pavement functions as a high quality base of support for the
new pavement, so there are similarities to conventional whitetopping.
Bonded concrete overlays have also been constructed. For these overlays,
the existing concrete pavement is carefully prepared to facilitate bond. These
measures are discussed in detail by Delatte et al. (1996a,b). These can be
as thin as 50 mm (2 in) because of the composite action with the existing
pavement. However, because any damage in the base concrete pavement will
reflect through the overlay, bonded concrete overlays are limited to exist-
ing pavement in good condition. This is probably the main reason that these
overlays remain rare – they are only suitable for pavements in relatively
good condition, and agencies are reluctant to invest in these pavements and
tend to allocate funds to pavements in worse condition. The other reason
they are rare is that if bond is not achieved, the thin overlays will fail rapidly.
A third type of concrete overlay on concrete pavement, the partially
bonded overlay, has been used in the past. For these overlays, no special
measures are taken to either prevent or achieve bond – the new concrete
is simply placed on top of the old. Some of these overlays were US Army
Corps of Engineers airfields, with thick overlays placed over thin existing
pavements. As a result, the contribution of the existing pavement may have
been very small. There seems to be very little recent construction of partially
bonded concrete overlays. In theory, at least, partially bonded overlays
would seem to be susceptible to reflective cracking.
Prestressed and precast concrete pavement
All conventional concrete pavements rely on the flexural strength of the
concrete to resist traffic loads over time. By using prestressing tendons to
induce a net compressive force in the pavement section it is possible to
considerably decrease the thickness of the pavement, because the traffic
loads must overcome the compressive stress before inducing a net tensile
stress and flexural fatigue into the pavement.
In addition to prestressed pavements for original construction or overlays,
precast concrete sections with either conventional or prestressed reinforce-
ment have been used as full depth patches. Precast sections may be left in
place as a permanent pavement, or may be temporary to allow traffic until
a permanent full depth patch is placed.
Pasko (1998) stated
prestressed concrete was introduced in the late 1940s and was used first
in airport pavements. About 1959, two-way prestressed slabs were used
Types of concrete pavements 39
at Biggs military airfield in Texas. The 24-in (610-mm) plain pavement
was replaced with 9-in (230-mm) post-tensioned slabs. Unfortunately,
the fear of the unknown, the need to use more skilled labor, and the
reluctance of mile-a-day slipform contractors to embrace this unproven
technology have held this concrete-saving technology back. About a
dozen highways with prestressed concrete pavements of various designs
were built in the United States between 1970 and 1990.
The first known prestressed test highway pavement was a short section in
Delaware in 1971. Other demonstration projects were at Dulles Airport,
along with two in Pennsylvania (Huang 2004: 16).
Another demonstration project, an unbonded overlay at Chicago O’Hare
International Airport, on Runway 8R-27L, was documented in the FAA
Engineering Brief No. 24. The base pavement was 305 mm (12 in) thick
CRCP on a 457 mm (18 in) thick crushed limestone base. The prestressed
overlay was 203 mm (8 in) thick on the western half and 228 mm (9 in)
thick on the eastern half, based on Boeing 747 aircraft. The dimensions
of the overlay were 244 m (800 ft) by 46 m (150 ft). The pavement was
prestressed in both the longitudinal and transverse directions (FAA 1981).
The 1993 AASHTO Pavement Design Guide discusses the design of pre-
stressed pavements. Prestressed pavement’s potential advantages include
more efficient use of construction materials (due to reduced pavement thick-
ness) and fewer joints and cracks, with reduced maintenance and longer
pavement life. Items addressed include:
• The pavement may be prestressed only longitudinally (with the pave-
ment unreinforced or conventionally reinforced transversely), pre-
stressed both longitudinally and transversely, or prestressed at an angle.
• Although prestressed pavement should work with low strength support,
fairly high strength subbases of 54 MPa/m (200 psi/in) or more have
generally been used.
• Much longer slabs may be used than conventional pavements – gener-
ally on the order of 122 m (400 ft) although slabs as long as 300 m
(1,000 ft) have been built in Europe.
• Prestress levels are typically 689–2,070 kPa (100–300 psi) in the longi-
tudinal direction and 0–1,380 kPa (0–200 psi) in the transverse direc-
• Typical tendons are 15 mm (0.6 in) strand stressed to 80 percent of
yield, spaced at two to four times slab thickness longitudinally and
three to six times slab thickness transversely.
• Because little is known about fatigue of prestressed pavements, and
because little warning may precede failure, designers should use con-
servative fatigue safety factors.